Features of the crystal structure and surface of superprotonic conductor caesium hydrogen sulfate phosphate.
Makarova, Irina P.; Isakova, Natalia N.; Kalyukanov, Andrey I.; Gainutdinov, Radmir V.; Tolstikhina, Alla L.; Komornikov, Vladimir A.; Acta crystallographica Section B, Structural science, crystal engineering and materials 80 (2024) –; doi:10.1107/S2052520624003470

data_2312502
_publ_section_title
;
 Features of the crystal structure and surface of superprotonic conductor
 caesium hydrogen sulfate phosphate.
;
_journal_coeditor_code           LO5120SUP1
_journal_issue                   3
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_paper_doi               10.1107/S2052520624003470
_journal_volume                  80
_journal_year                    2024
_chemical_compound_source        'synthesised by authors'
_chemical_formula_analytical     'Cs4 H5 O16 P S3'
_chemical_formula_iupac          'Cs4 H5 O16 P S3'
_chemical_formula_moiety         'Cs4 H5 O16 P S3'
_chemical_formula_structural     'Cs4 H5 O16 P S3'
_chemical_formula_sum            'Cs4 H5 O16 P S3'
_chemical_formula_weight         919.8
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.12(2)
_cell_angle_gamma                90
_cell_formula_units_Z            3
_cell_length_a                   19.95(3)
_cell_length_b                   7.856(9)
_cell_length_c                   8.980(10)
_cell_measurement_reflns_used    1501
_cell_measurement_temperature    293
_cell_measurement_theta_max      41.94
_cell_measurement_theta_min      3.09
_cell_volume                     1386(3)
_diffrn_ambient_temperature      293
_diffrn_detector                 MAR345n
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.98
_diffrn_measurement_device       diffractometer
_diffrn_measurement_device_type  MOND
_diffrn_measurement_method       scans
_diffrn_radiation_monochromator  'PG(002)/PG(002) double monochromator'
_diffrn_radiation_probe          neutron
_diffrn_radiation_source         neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.06
_diffrn_reflns_av_R_equivalents  0.0848
_diffrn_reflns_av_unetI/netI     ' '
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            1950
_diffrn_reflns_reduction_process ' '
_diffrn_reflns_theta_full        41.94
_diffrn_reflns_theta_max         41.94
_diffrn_reflns_theta_min         3.09
_diffrn_source                   neutron
_diffrn_standards_decay_%        ' '
_diffrn_standards_interval_count ' '
_diffrn_standards_interval_time  ' '
_diffrn_standards_number         ' '
_exptl_absorpt_coefficient_mu    0.0
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.306
_exptl_crystal_description       piece
_exptl_crystal_F_000             328.6
_exptl_crystal_size_max          2.5
_exptl_crystal_size_mid          1.0
_exptl_crystal_size_min          0.8
_refine_diff_density_max         0.23
_refine_diff_density_min         -0.23
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    3.54
_refine_ls_goodness_of_fit_ref   3.54
_refine_ls_hydrogen_treatment    mixed
_refine_ls_number_constraints    0
_refine_ls_number_parameters     106
_refine_ls_number_reflns         525
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1119
_refine_ls_R_factor_gt           0.1119
_refine_ls_shift/su_max          0.0834
_refine_ls_shift/su_mean         0.0120
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0004F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1336
_refine_ls_wR_factor_ref         0.1336
_reflns_number_gt                525
_reflns_number_total             1041
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            lo5120sup1.cif
_cod_data_source_block           I
_cod_database_code               2312502
_cod_database_fobs_code 2312502